Low-loss silicon nitride waveguide hybridly silicon nitride waveguide hybridly integrated with...
Embed Size (px)
Transcript of Low-loss silicon nitride waveguide hybridly silicon nitride waveguide hybridly integrated with...
Low-loss silicon nitride waveguide hybridly integrated with colloidal quantum dots
Weiqiang Xie,1,2,* Yunpeng Zhu,1,2 Tangi Aubert,2,3 Steven Verstuyft,1,2 Zeger Hens,2,3 and Dries Van Thourhout1,2
1Photonics Research Group, Department of Information Technology, Ghent University-IMEC, Gent B-9000, Belgium 2Center for Nano and Biophotonics, Ghent University, B-9000 Ghent, Belgium
3Physics and Chemistry of Nanostructures, Ghent University, B-9000 Ghent, Belgium *[email protected]
Abstract: Silicon nitride waveguides with a monolayer of colloidal quantum dots embedded inside were fabricated using a low-temperature deposition process and an optimized dry etching step for the composite layers. We experimentally demonstrated the luminescence of the embedded quantum dots is preserved and the loss of these hybrid waveguide wires is as low as 2.69dB/cm at 900nm wavelength. This hybrid integration of low loss silicon nitride photonics with active emitters offers opportunities for optical sources operating over a very broad wavelength range. 2015 Optical Society of America OCIS codes: (130.0130) Integrated optics; (230.7370) Waveguides; (160.4236) Nanomaterials.
References and links 1. E. S. Hosseini, S. Yegnanarayanan, A. H. Atabaki, M. Soltani, and A. Adibi, High quality planar silicon nitride
microdisk resonators for integrated photonics in the visible wavelength range, Opt. Express 17(17), 1454314551 (2009).
2. Q. Li, A. A. Eftekhar, M. Sodagar, Z. Xia, A. H. Atabaki, and A. Adibi, Vertical integration of high-Q silicon nitride microresonators into silicon-on-insulator platform, Opt. Express 21(15), 1823618248 (2013).
3. S. Romero-Garca, F. Merget, F. Zhong, H. Finkelstein, and J. Witzens, Silicon nitride CMOS-compatible platform for integrated photonics applications at visible wavelengths, Opt. Express 21(12), 1403614046 (2013).
4. A. Z. Subramanian, P. Neutens, A. Dhakal, R. Jansen, T. Claes, X. Rottenberg, F. Peyskens, S. Selvaraja, P. Helin, B. Du Bois, K. Leyssens, S. Severi, P. Deshpande, R. Baets, and P. Van Dorpe, Low-loss singlemode PECVD silicon nitride photonic wire waveguides for 532-900 nm wavelength window fabricated within a CMOS pilot line, IEEE Photonics J. 5(6), 2202809 (2013).
5. D. J. Moss, R. Morandotti, A. L. Gaeta, and M. Lipson, New CMOS-compatible platforms based on silicon nitride and Hydex for nonlinear optics, Nat. Photonics 7(8), 597607 (2013).
6. M. Eichenfield, R. Camacho, J. Chan, K. J. Vahala, and O. Painter, A picogram- and nanometre-scale photonic-crystal optomechanical cavity, Nature 459(7246), 550555 (2009).
7. M. Khan, T. Babinec, M. W. McCutcheon, P. Deotare, and M. Loncar, Fabrication and characterization of high-quality-factor silicon nitride nanobeam cavities, Opt. Lett. 36(3), 421423 (2011).
8. K. Luke, A. Dutt, C. B. Poitras, and M. Lipson, Overcoming SiN film stress limitations for high quality factor ring resonators, Opt. Express 21(19), 2282922833 (2013).
9. X. Tu, J. Song, T. Y. Liow, M. K. Park, J. Q. Yiying, J. S. Kee, M. Yu, and G. Q. Lo, Thermal independent silicon-nitride slot waveguide biosensor with high sensitivity, Opt. Express 20(3), 26402648 (2012).
10. L. Martiradonna, T. Stomeo, M. De Giorgi, R. Cingolani, and M. De Vittorio, Nanopatterning of colloidal nanocrystals emitters dispersed in a PMMA matrix by e-beam lithography, Microelectron. Eng. 83(49), 14781481 (2006).
11. Y. K. Olsson, G. Chen, R. Rapaport, D. T. Fuchs, V. C. Sundar, J. S. Steckel, M. G. Bawendi, A. Aharoni, and U. Banin, Fabrication and optical properties of polymeric waveguides containing nanocrystalline quantum dots, Appl. Phys. Lett. 85(19), 4469 (2004).
12. I. Surez, H. Gordillo, R. Abargues, S. Albert, and J. Martnez-Pastor, Photoluminescence waveguiding in CdSe and CdTe QDs-PMMA nanocomposite films, Nanotechnology 22(43), 435202 (2011).
13. C. A. Foell, E. Schelew, H. Qiao, K. A. Abel, S. Hughes, F. C. J. M. van Veggel, and J. F. Young, Saturation behaviour of colloidal PbSe quantum dot exciton emission coupled into silicon photonic circuits, Opt. Express 20(10), 1045310469 (2012).
14. M. Humer, R. Guider, W. Jantsch, and T. Fromherz, Integration, photostability and spontaneous emission rate enhancement of colloidal PbS nanocrystals for Si-based photonics at telecom wavelengths, Opt. Express 21(16), 1868018688 (2013).
15. S. Gupta and E. Waks, Spontaneous emission enhancement and saturable absorption of colloidal quantum dots coupled to photonic crystal cavity, Opt. Express 21(24), 2961229619 (2013).
#235693 - $15.00 USD Received 5 Mar 2015; revised 24 Apr 2015; accepted 27 Apr 2015; published 29 Apr 2015 2015 OSA 4 May 2015 | Vol. 23, No. 9 | DOI:10.1364/OE.23.012152 | OPTICS EXPRESS 12152
16. A. Qualtieri, F. Pisanello, M. Grande, T. Stomeo, L. Martiradonna, G. Epifani, A. Fiore, A. Passaseo, and M. De Vittorio, Emission control of colloidal nanocrystals embedded in Si3N4 photonic crystal H1 nanocavities, Microelectron. Eng. 87(58), 14351438 (2010).
17. A. Gorin, A. Jaouad, E. Grondin, V. Aimez, and P. Charette, Fabrication of silicon nitride waveguides for visible-light using PECVD: a study of the effect of plasma frequency on optical properties, Opt. Express 16(18), 1350913516 (2008).
18. Y. Justo, I. Moreels, K. Lambert, and Z. Hens, Langmuir-Blodgett monolayers of colloidal lead chalcogenide quantum dots: morphology and photoluminescence, Nanotechnology 21(29), 295606 (2010).
19. B. De Geyter, K. Komorowska, E. Brainis, P. Emplit, P. Geiregat, A. Hassinen, Z. Hens, and D. Van Thourhout, From fabrication to mode mapping in silicon nitride microdisks with embedded colloidal quantum dots, Appl. Phys. Lett. 101(16), 161101 (2012).
20. R. A. Morgan, Plasma Etching in Semiconductor Fabrication (Elsevier Press, 1985), Chap. 3. 21. J. W. Coburn, Insitu Auger electron spectroscopy of Si and SiO2 surfaces plasma etched in CF4H2 glow
discharges, J. Appl. Phys. 50(8), 52105213 (1979). 22. J. W. Coburn and H. F. Winters, Plasma etchinga discussion of mechanisms, J. Vac. Sci. Technol. 16(2),
391403 (1979). 23. V. Srivastav, R. Pal, and H. P. Vyas, Overview of etching technologies used for HgCdTe, Opto-Electron. Rev.
13(3), 197211 (2005).
Silicon nitride (SiN) exhibits transparency from the visible to the mid-infrared and has a fairly high optical index (~2.0), making it suitable for various photonic applications including integrated photonic circuits , nonlinear optics , high quality optical cavities , and on-chip biosensing . On the other hand, because of its dielectric nature, the SiN platform is thus far limited to passive devices and a light source such as a laser or a single photon emitter integrated in this platform is highly desired. Colloidal quantum dots (QDs), with their efficient luminescence, tunable from the visible to the infrared wavelength, potentially could be used as the emitters in photonic applications. In fact, colloidal QDs have already been integrated with various types of photonic integrated circuits (PIC), including polymer matrix and waveguides , silicon photonic circuits [13, 14] and SiN nanocavities . In all these examples, the QDs were either stabilized in a polymer matrix or directly dispersed on the surface of the devices. Given the drawbacks of the polymers used (low index contrast, unknown long term stability) and the instability of the QDs themselves when they are left exposed, there is a need for the integration of colloidal QDs with an all inorganic low-loss PIC-platform whereby the QDs are fully encapsulated. Furthermore, given the wide tunability of colloidal QDs e.g. by changing their diameter and/or the materials used it is important also the waveguide platform used is capable of handling a wide range of wavelengths. SiN provides this wide tunability and therefore its integration with QDs forms a promising route to achieve this goal. For practical applications, it is important that the QDs are well stabilized within the SiN layers used for realizing the waveguides, using a process that does not affect the optical properties of the QDs and while still allowing realizing high performance optical circuits. In addition it is important that the geometrical pattern of the embedded QD film and its location can be controlled precisely with respect to the targeted optical devices. Although, colloidal QDs have been embedded in SiN photonics , there is still a lack of quantitative evaluation of this hybrid photonic platform in terms of optical losses and optimal fabrication process.
In this work, we developed a low-loss hybrid SiN-QD photonic platform based on a low-temperature (120-270C) plasma enhanced chemical vapor deposition (PECVD) process. By using an optimized dry etching process, we fabricated waveguides with a close-packed monolayer of colloidal QDs embedded into two layers of SiN, of which the top layer was deposited at 120C to maximally preserve the luminescence of the QDs. At 900nm wavelength a loss as low as 2.69dB/cm is demonstrated for these hybrid waveguides. Since only standard lithography and direct top-down etching is utilized here, one could envisage leveraging mature complementary metal-oxide-semiconductor (CMOS) technology for the realization of active SiN devices, e.g. high quality factor cavities with embedded QDs. Therefore the present hybrid SiN-QD platform provides a promising solution for the integration of optical emitters with the fully inorganic SiN photonic platform.
#235693 - $15.00 USD Received 5 Mar 2015; revised 24 Apr 2015; accepted 27 Apr 2015; published 29 Apr 2015 2015 OSA 4 May 2015 | Vol. 23, No. 9 | DOI:10.1364/OE.23.012152 | OPTICS EXPRESS 12153
2. Mask design and fabrication
The test pattern